# Viscoelastic Indentation and Resistance to Motion of Conveyor Belts

```Viscoelastic Indentation and Resistance to Motion of Conveyor Belts
using a Generalized Maxwell Model of the Backing Material
Thomas J. Rudolphi a and Allen V. Reicks b
a
Department of Aerospace Engineering, Iowa State University, Ames, IA
b
Design Manager, Overland Conveyor, Inc., Denver, CO
Abstract
A one-dimensional Winkler foundation and a generalized viscoelastic Maxwell solid
model of the belt backing material are used determine the resistance to motion of a
conveyor belt over idlers. The viscoelastic material model is a generalization of the
three-parameter Maxwell model that has previously been used to predict the effective
frictional coefficient of the rolling motion. Frequency, or loading rate, and temperature
dependence of the material properties are incorporated with the time/temperature
correspondence principle of linear viscoelastic materials. As a consequence of the
Winkler foundation model, a normalized indentation resistance is independent of the
primary belt system parameters – carrying weight per unit width, idler diameter and
backing thickness - as is the case for a three-parameter viscoelastic model. Example
results are provided for a typical rubber compound backing material and belt system
parameters.
Keywords: Rolling contact; Viscoelastic layer; Generalized Maxwell model; Winkler
foundation; Indentation resistance
Rudolphi/Reicks
2/22/2006
Introduction
Advances in rubber materials, belt fabrication and conveyor system technology,
together with demands for larger systems to transport bulk granular materials, put a
premium on efficient system design. The power to drive large conveyor systems is a
critical design parameter, due to energy costs over the life of the system. Dissipative
energy losses due to inelastic deformation and indentation of the belt covering, or
“backing”, material on a belt as it passes over each idler of the system is generally
considered to be one of, if not the, dominant loss mechanism in the system. Hager and
Hintz1 estimate this source of power loss to be as much or greater than 60% of the total.
Predictive analytical models of this loss are thus important to designers of such systems
and several models have been developed and used.
The model of rolling resistance developed herein follows and builds on the work of
several authors, including May, Morris and Atak2, Jonkers3, Spaans4, Lodewijks5,6 and
Johnson7. These authors model the indentation of the idler into the backing as a onedimensional stress/strain situation with the idler considered rigid and the backing as a
Winkler foundation on a rigid base. Thus the compressed fibers, through the depth of the
backing, act independently such that there is no accounting for shear in the deformation
process. The full two-dimensional models of Hunter8 and Morland9 account for shear
deformation, although they presume the backing to be a viscoelastic half-space, as
opposed to having a finite depth, and require the solution of dual integral Equations to
satisfy the contact equilibrium and deformation conditions.
More importantly, however, in the analyses mentioned above, the viscoelastic
material behavior is presumed to be that of a simple, three-parameter Maxwell solid.
However, rubber materials commonly used for backing on conveyor belts are highly
temperature and load-rate dependent, so a useful viscoelastic constitutive model must
accurately account for these effects. The three parameter model is extremely range
limited, in both temperature and rate effects, to capture real viscoelastic behavior. In the
present analysis, the three-parameter constitutive model is generalized to arbitrary 2 N + 1
parameters, and used in combination with the Winkler foundation deformation model.
Thermal and rate effects are incorporated through the well-accepted time/temperature
superposition principle 9,10 of linear viscoelasticity to provide a simple, yet sufficiently
comprehensive model of the deformation and material response, to capture realistic
The Indentation Resistance Model
For a linear viscoelastic material and a one-dimensional state of stress, the stress
relaxation formula for a prescribed strain history is determined by,10
σ (t ) = Ψ (t )ε (0 ) + ∫ Ψ (t − s )ε&amp; (s )ds
+
t
(1)
0
where Ψ (t ) is the stress relaxation function, ε&amp; ≡ dε dt is the strain rate and σ (t ) is the
stress at time t . For the present analysis the time t = 0 is taken to be that instant at
which the belt first contacts the idler so that ε 0 + = 0 .
( )
Rudolphi/Reicks
2/22/2006
v
Backing material
h
z
(x, z )
δ
x
x=a
x = −b
ω
R
Idler
Figure 1. Indentation of the idler into the backing material and geometric parameters.
Following the work and general notational conventions of Jonkers3, Spaans4,
Lodewijks5,6 and Johnson7, the kinematics of the deformation process for the belt backing
passing over an idler at uniform speed v is shown in Figure 1. At a constant speed the
deformation process is essentially steady state with respect to the Eulerian coordinate
x = a − vt , where t denotes time and a the point of contact of the belt and idler ( x is
fixed with respect to the idler, but not rotating with it). The problem of steady motion
may then be cast in terms of the coordinate x as opposed to the explicit time t through
the above transformation.
For a small maximum indentation depth δ compared to the idler radius R , or
δ R &lt;&lt; 1 , the indentation amount at a point x on the surface of the idler is approximated
by a parabola such that z = δ − x 2 2 R , where δ = a 2 2 R . Hence the compressional
strain of the backing material at the coordinate x , modeled as a Winkler foundation or
independent linear elements through the backing, is
z 1
1
a2 − x2
ε = = δ − x 2 2R =
(2)
h h
2 Rh
Using the translating coordinate speed relationship, x&amp; = −v , so z&amp; = −2 xx&amp; / 2 R = xv / R , the
strain rate, or time derivative of Equation (2), becomes ε&amp; = z&amp; h = vx Rh . With this strain
rate, the compressional stress between idler and belt, from Equation (1), may be
expressed as a function of t or as a steady function of x ,
(
Rudolphi/Reicks
)
(
)
2/22/2006
v
(a − vs )ds = − 1 ∫ Ψ⎛⎜ ξ − x ⎞⎟ξ dξ
(3)
Rh
Rh a ⎝ v ⎠
0
Now, for a given material relaxation function Ψ , this Equation can, in principle, be
integrated to explicitly determine the contact stress profile between the belt and the idler
as depicted in Figure 2. However, the contact length a + b , or both the point of first
contact a and the point of departure b , are undetermined; they depend on the load or net
t
x
σ = ∫ Ψ (t − s )
− σ (x )
z
x
x = −b
x=a
R
Idler
Figure 2. Contact stress distribution between idler and backing.
force between the belt and idler, and hence, as in most situations involving contacting
materials, this problem is geometrically nonlinear.
At equilibrium, the load W (force per unit width across the idler) and the resultant of
the stress distribution must be in balance such that
a
W = ∫ σ ( x ) dx
(4)
−b
To determine a and b , Equations (3) and (4) must be satisfied simultaneously, but an
explicit solution is not possible. However, as shown by Lodewijks5, a simple iterative
procedure can be used to balance the load and the contact length, determining both a and
b , given the load W .
Once the stress profile and contact length is determined, the moment M of the stress
distribution about the center of the idler is
Rudolphi/Reicks
2/22/2006
a
M = ∫ xσ ( x ) dx
(5)
−b
Then the resistance force to rolling is M R and the coefficient of rolling resistance, or
equivalent Coulomb drag coefficient &micro; , is
a
M
1
=
&micro;=
RW R
∫ xσ (x )dx
−b
a
(6)
∫ σ (x )dx
−b
In the following section, the above Equations are evaluated, incorporating the generalized
material model, to provide a closed form model for the indentation resistance.
The Generalized Maxwell Material Model
For rubber compounds used as backing for belt conveyors, it is common to use the simple
three-parameter Maxwell constitutive model. For realistic backing materials, however,
the three parameter model is not capable of representing viscoelastic behavior over a
range of temperatures and loading rates. The three parameter model is easily generalized
to 2 N + 1 parameters as shown in Figure 3, or to what is sometimes called the Zenar
η1
η2
η3
E1
E2
E3
L η
N
L η
i
E0
Ei
EN
L
L
Figure 3. The mechanical elements of the Maxwell solid model.
model. The constants Ei and η i represent the various elastic and dissipative viscous
elements of the model and the constant E 0 is referred to as the long term or equilibrium
modulus.
According to this generalized 2 N + 1 parameter model, the stress response function
is given by the Prony series11
N
Ψ (t ) = E 0 + ∑ Ei e −t / τ
i
(7)
i =1
where τ i = η i / Ei are the characteristic periods of the various dissipative elements of the
mechanical model. Insertion of this response function into Equation (3) for the stress,
including the transformation t = (a − x ) / v , one has,
Rudolphi/Reicks
2/22/2006
N
⎤
⎡
(8)
Rhσ (t ) = − ∫ ⎢ E 0 + ∑ Ei e −(ξ − x ) / vτ i ⎥ξ dξ
i =1
⎦
a ⎣
Then, similar to the 3-parameter model, each term of series in this Equation can be
integrated to arrive at the result,
1⎛ x⎞
⎡
⎛
− ⎜ 1− ⎟ ⎞
E0 ⎛
Rh
x ⎞⎛
x⎞ N
x ⎞⎤
⎛
ki ⎝ a ⎠ ⎟
⎜
⎢
(
)
x
E
k
k
e
σ
(
)
1
1
1
1
1
(9)
+
+
−
−
−
+
=
−
⎜
⎟⎥
⎟ ∑ i i
⎜
⎟⎜
i
⎜
⎟ ⎝ a ⎠⎥
2 ⎝ a ⎠⎝ a ⎠ i =1
a2
⎢
⎝
⎠
⎣
⎦
where k i = vτ i / a are the Deborah (wave) numbers corresponding to the N element pairs
of the material model.
Now, introducing the non-dimensional length parameter ς = b / a , and equating the
stress of Equation (8) to zero at x = −b provides the condition,
N
E0
(1 + ς )(1 − ς ) + ∑ Ei k i k i − ς − (1 + k i )e −(1+ς ) ki = 0
(10)
2
i =1
For given material parameters, the solution of this Equation would provide only the ratio
ς = b / a , not a or b explicitly. The additional condition that must be satisfied is
Equation (4), which, when integrated and also expressed in terms of ς is
N
E0
Rh
⎧1
⎫
3
=
+
−
+
W
2
3
ς
ς
Ei k i ⎨ 1 − ς 2 − k i (1 + k i ) 1 − e −(1+ς ) / ki − (1 + ς ) ⎬ (11)
∑
3
6
a
⎩2
⎭
i =1
Then, for given material parameters E i , k i , and belt system parameters W , R and h , the
values of ς and a , which satisfy both Equations (10) and (11), will be in equilibrium
with the load W . The simultaneously solution is readily accomplished numerically by a
simple iterative procedure:
(a) Initialize a guess for ς and solve Equation (11) for a .
(b) Use this value of a to determine the material parameters k i = vτ i / a .
x
[
(
)
(
]
[
)
(
)
]
(c) With these values of k i and E i , solve (numerically) Equation (10) for ς .
(d) Use the updated value of ς , replace the initial guess of step (a) and continue
repetition of steps (a), (b) and (c) until ς converges to a predetermined accuracy.
Following this iterative process to determine an accurate value of ς = b a , a and
b , Equation (5) can then be evaluated to get the moment of the stress distribution. Thus,
E a4
M = 0 2 1 − 2ς 2 + ς 4 +
8R h
(12)
N
Ei a 4 ki ⎡ 3 ki
1
− (1+ς ) / ki ⎤
2
3
∑
2
⎢ki − 2 1 + ς + 3 1 + ς − ki (1 + ki )(ki + ς )e
⎥
⎦
i =1 R h ⎣
The indentation resistance coefficient then follows from Equations (6), (11) and (12).
Combining these Equations in such a way as to eliminate the explicit appearance of
the contact length parameter a , Equation (6) can be written as
(
)
(
) (
)
1/ 3
1 ⎛ M ⎞ ⎛ Wh ⎞
M*
⎟
&micro; = ⎜ ⎟ = ⎜⎜
(13)
R ⎝ W ⎠ ⎝ E 0 R 2 ⎟⎠ (F * )4 / 3
where the non-dimensional functions F * and M * have been introduced and are given by,
Rudolphi/Reicks
2/22/2006
F * (ς ) ≡
]
(14)
1
1 − 2ς 2 + ς 4
8
N
⎛E ⎞ ⎡
k
1
⎤
+ ∑ ⎜⎜ i ⎟⎟k i ⎢k i3 − i 1 + ς 2 + 1 + ς 3 − k i (1 + k i )(k i + ς )e −(1+ς ) / ki ⎥
2
3
⎣
⎦
i =1 ⎝ E 0 ⎠
(15)
N
⎛E
1
2 + 3ς − ς 3 + ∑ ⎜⎜ i
6
i =1 ⎝ E 0
M * (ς ) ≡
(
)
(
[
⎞ ⎧1 − ς 2
⎫
⎟⎟k i ⎨
− k i (1 + k i ) 1 − e −(1+ς ) / ki − (1 + ς ) ⎬
⎭
⎠ ⎩ 2
(
)
)
(
)
(
)
In both these functions, the moduli have been normalized to E 0 , giving rise to the ratio
(
(E i
E 0 ) in each expression and introduces the non-dimensional factor Wh E 0 R 2
coefficient of &micro; in Equation (13).
)
1/ 3
as a
Equation (12) then shows the direct dependence of &micro; on (Wh R 2 ) , as is a direct
consequence of the Winkler foundation model and consistent with the results of the three
parameter material models of other3-6. Inclusion of E 0 in this factor renders it nondimensional. Reflecting this factor, a normalized indentation factor F is defined by,
1/ 3
−1 / 3
⎛ Wh ⎞
M*
⎟
=
(15)
F ≡ &micro; ⎜⎜
2 ⎟
(F * )4 / 3
⎝ E0 R ⎠
It is noted that since this normalized indentation factor is the ratio of two terms that
depend only on the material parameters k i and Ei , so after the load dependent factor ς
has been determined by the iterative process described above, then F is solely a function
of the backing material viscoelastic properties. As such, F is independent of the belt
system parameters W , h and R , unlike the coefficient &micro; , is essentially a material
property from which the indentation resistance can be determined for any W , h and R .
Temperature Dependent Material Modeling
Mechanical properties of a viscoelastic material are typically measured by cyclicallyimposed deformation tests on standard specimens in simple extension, shear, bending or
torsion at controlled temperatures and at relatively low frequencies to avoid inertial
effects. By testing over a wide temperature range but limited frequencies, and using the
superposition principle, which relates time (equivalently frequency or speed) and
temperature effects, one can extrapolate to frequencies or load rates considerably beyond
those of the test. This theoretical rheological model for viscoelastic materials, supported
by experimental measurements, and postulating the equivalence of temperature and time
effects, is known as the time/temperature superposition principle9,10. According to this
principle, if T denotes temperature and T0 a reference temperature, then a material
property at time t and temperature T is equivalent to that at time aT t and temperature T0 ,
where aT is a “shift” parameter in time so that aT = aT (T , T0 ) . A commonly used
expression for aT , applicable to amorphous polymers at temperatures above the glass
transition temperature Tg , due to Williams, Landel and Ferry12 and referred to as the
WLF Equation, is the logarithmic form, log(aT ) = C1 (T − T0 ) [C 2 + (T − T0 )] , where C1
and C 2 are constants determined empirically from data.
Rudolphi/Reicks
2/22/2006
Alternately, for data taken from cyclical or frequency controlled strain experiments,
an empirical representation of the time/temperature shift parameter aT may be
determined by overlaying, through shifts in the frequency, the temperature dependent
modulus data onto a “master” curve. The required frequency shift, on a logarithmic
scale, for data at each test temperature, to produce the overlay determines the equivalent
of the WLF Equation, or may be taken the basic temperature/frequency relationship of
the superposition principle. This master curve approach is used here to relate temperature
and frequency, or load rate effects, within the generalized Maxwell material model. So
instead of the above functional form for aT of the WLF Equation with only two
constants, the relationship between aT and temperature T is taken as,
n
log(aT ) = ∑ ai T i = a 0 + a1T + a 2T 2 + L + a nT n
(16)
i =0
and the constants ai are determined by a least squares curve fitting process in the
construction of the master curve for the material.
Experimental measurement of the mechanical properties of polymeric materials is
most often done by subjecting specimens to cyclic strain programs at fixed temperatures
and over a limited range of frequencies. For a sinusoidal strain history of the form
ε = ε 0 sin (ωt ) , where ω is the circular frequency and ε 0 the amplitude, and after an
initial transitory state, the stress follows the strain in frequency, but at a delayed phase.
For elastic material, the stress and strain are in phase, but for viscoelastic materials there
is a delayed response, and it is convenient to express this relationship in the form10,
[
σ (t ) = E * (ω )ε (t ) = E ′(ω )2 + E ′′(ω )2
]
1/ 2
ε 0 sin (ωt + δ )
(17)
*
where E is the magnitude of the complex modulus with real and imaginary components
E ′(ω ) and E ′′(ω ) , called the storage and loss moduli, respectively, and
δ (ω ) = E ′′(ω ) / E ′(ω ) is the phase angle or lag of stress behind strain. For the generalized
Maxwell model, the storage and loss moduli are related to the mechanical elements of the
model shown in Figure 3 by 11,
N
E ′(ω ) = E 0 + ∑ Ei
i =1
ω 2τ i2
1 + ω 2τ i2
(18)
and
ωτ i
(19)
1 + ω 2τ i2
i =1
where Ei are now the discrete or spectral values of the Maxwell model and τ i = η i Ei
are the periods of the various elements.
Implicit in material properties E ′(ω ) and E ′′(ω ) is the dependence on temperature.
In the frequency domain, the superposition principle relates properties at temperatures
and frequencies according to the relationships
E ′(ω , T ) = E ′(aT ω , T0 ), E ′′(ω , T ) = E ′′(aT ω , T0 )
(20)
From these Equations, which represent the material’s master curves of E ′(ω ) and
E ′′(ω ) , one can extrapolated to frequencies, and hence loading rates, considerably
N
E ′′(ω ) = ∑ Ei
Rudolphi/Reicks
2/22/2006
beyond those of the test data. For a given belt speed v , the relationship between load rate
and frequency is taken to be
πv
(21)
ω=
a+b
which derives from the presumption that an element of the material of the backing passes
through a half-cycle of loading during the contact period. This Equation, which couples
the material properties and contact length, and hence the material properties to the
deformation and equilibrium Equations, through the iterative process outlined previously
for Equations (10) and (11) in the establishment of a and b .
Figures 4 and 5 show the combination master curves and shift factor of the shear moduli
G ′(ω ) = E ′(ω ) 3 and G ′′(ω ) = E ′′(ω ) 3 for a typical, incompressible, belt backing
material.
The tests were performed with a Rheometric Scientific ARES mechanical
spectrometer in a twisting/shear mode on flat specimens with approximate dimensions of
35x13x4mm. Data were taken test over a temperature range of − 60 o to + 70 o C at about
10 o increments and frequencies from 0.01 to 15 Hz with about 13 equally spaced
increments on a logarithmic scale. The shift factor aT of Figure 5 was developed
according to Equation (16), from the data at each temperature increment, starting from a
chosen reference temperature.
Storage (G') and Loss (G'') Moduli [Pa]
10
10
10
10
10
10
Storage (G') and Loss (G'') Moduli vs. Frequency
10
Shifted G' data
Shifted G'' data
Master poly (n = 13), G'
Master poly (n = 13), G''
G' from spectrum
G'' from spectrum
9
8
7
6
5
10
-10
10
-5
0
10
10
Frequency [Hz]
5
10
10
10
15
Figure 4. Master curve for a typical belt backing material.
Rudolphi/Reicks
2/22/2006
The reference temperature for this curve is 0 o C , which is where aT equals 1 of Figure 5,
and a polynomial of order 5 is shown on the curve with the discrete aT values of the
fitting process, as prescribed by Equation (16).
10
Temperature/Frequency Shift Factor vs. Temerature
15
Least squares data fit
Polynomial (n = 5) fit
10
5
aT
10
10
10
10
10
0
-5
-10
-60
-40
-20
0
20
Temperature [C]
40
60
80
Figure 5: Frequency/temperature shift factor.
For this material, as characterized by the master curve and frequency/temperature
shift factor, the discrete 2 N + 1 parameters of the Maxwell model, i.e., values of Ei and
η i of Equations (17) and (18) are also determined. This amounts, equivalently, to the
determination of the discrete spectrum of the material, where Equations (18) and (19)
represent the discrete versions of comparable continuous transforms.
Determination of these discrete spectral values has been the focus of much research
and various techniques and mathematical fitting processes – Tschoegl13 and Emri and
Tschoegl14. Neural networks and genetic algorithms have also been employed to “best
fit” both Ei and η i , or equivalently Ei and τ i , from given data as in Figure 4.
Alternately, a common and fairly simple approach is to fix the periods τ i = 1 ω i at values
equally spaced on the log(ω ) scale (half-decade increments is sufficient 13) and then use a
least square curve fit to the “data” as calculated from the polynomial fit of the master
curve at the τ i = 1 ω i values over the range of the data. Here, a non-linear, non-negative,
least square method is used to fit the data. The non-negative constraint on the fitting
Rudolphi/Reicks
2/22/2006
process is not necessary, but eliminates the possibility of negative Ei coefficients, which
is not uncommon for this type of transform13.
Figure 6 shows the resulting spectral values that result from fitting the G ′ master
curve to Equation (18). The re-calculate values of G ′ and G ′′ that result from the
spectrum, through Equations (16) and (17) are shown in the original master curves in
Figure 4. Note that the re-calculated G ′ is accurate, since the spectrum is fit to this
“data”, but also the calculation of G ′′ from the spectrum derived from fitting G ′ is also
Discrete Spectrum of Storage Modulus G'
9
8
log(Spectral Strength) [Pa]
7
6
5
4
3
2
1
0
-15
-10
-5
0
5
10
log(τ [s])
Figure 6.
Discrete spectrum of the storage modulus G ′ .
accurate over the range of the data. Some deviation is evident at the frequency extremes,
but the consistency of the fit is evidence of the redundancy involved in the spectral
characterization of both Equations (16) and (17).
Indentation Resistance Calculations
With the discrete spectrum of Figure 6 as a characterization of a typical backing
material, the indentation resistance model of Equations (10) – (15) were evaluated for a
range of temperatures and belt speeds, and at typical values of system parameters:
W = 10 lb / in = 1751.3 N / m, h = 0.25 in = 0.00635 m R = 3 in = 0.0762 m . Belt speed,
being a function of time, relates also to temperature through the superposition principle,
Rudolphi/Reicks
2/22/2006
which allows for the construction of universal curves of &micro; and F , for any
temperature/speed combination when graphed as functions of vaT . Thus, Figures 7 and 8
give, respectively, the friction coefficient &micro; of Equation (13) and the non-dimensional
value F of Equation
(13).
4.5
x 10
-3
Friction Coefficient vs. Temperature Scaled Belt Speed
4
&micro; - friction coefficient
3.5
3
2.5
2
1.5
1
0.5
0
-5
10
10
0
10
5
10
10
v*aT (m/s)
Figure 7: Indentation resistance &micro; vs. scaled belt speed.
Rudolphi/Reicks
2/22/2006
Normalized Friction Coefficient vs. Temperature Scaled Belt Speed
0.1
0.09
0.08
F = &micro; /(Wh/E 0R2)1/3
0.07
0.06
0.05
0.04
0.03
0.02
0.01
0
-5
10
10
0
10
5
10
10
v*aT (m/s)
Figure 8. Normalized indentation resistance F vs. scaled belt speed.
These graphs are actually composites, or overlapping segments, of the calculation of &micro;
and F through the algorithm above, with the calculations performed through nested
loops through increments in the temperature T and speed v . When graphed against vaT ,
these resulting curves actually overlap, but the overlapping portions are only faintly
visible in the graphs, which is a consequence of the superposition principle. Thus,
Figures 7 and 8 are universal curves, implicit in temperature, i.e., applicable to all
temperatures in the range provided by the shift parameter aT of Figure 5.
Determination of specific values of &micro; or F from the curves of Figures 7 and 8, at
given values of the belt speed v and temperature T , is then done in conjunction with the
aT curve of Figure 5. Given T , one would first find the value of aT from Figure 5,
providing the ordinate vaT for the corresponding value of &micro; and F from Figures 7 and
8. Thus, for this material at a temperature of, say, T = −20 o C , Figure 5 provides a value
aT ≈ 10 3 , and at a speed of 2 m/s so that vaT = 2 &times; 10 3 m/s , the values of &micro; and F from
Figures 7 and 8 would be located on the curves just at about the peaks of the curves and
be about 0.0044 and 0.089 , respectively. As noted previously, utility of the nondimensional F of Figure 8 is that it pertains to systems with any values of W , h and R .
For the same material and calculations, Figure 9 shows the corresponding contact
length parameter ς = b / a as results from the iteration process at which the load W is in
equilibrium with the contact stress. It is noted here that a minimal value of ς occurs at
Rudolphi/Reicks
2/22/2006
vaT ≈ 10 3 m/s , which, not surprisingly, is the same speed/temperature at which the
indentation resistance factors &micro; and F attain their maximum values.
b/a vs. Temperature Scaled Belt Speed
1
0.95
ζ = b/a
0.9
0.85
0.8
0.75
0.7
0.65
-5
10
10
0
10
5
10
10
v*aT (m/s)
Figure 9. Contact length ratio vs. scaled frequency.
Discussion and Conclusions
A predictive model of the indentation and rolling resistance of a linear viscoelastic
material backing on a conveyor belt using a generalized Maxwell material model of the
backing material has been made. This represents a generalization of the three parameter
model that has traditionally been used for the calculation of the indentation resistance, but
which is capable of capturing the real polymeric behavior of rubber backings used on
large, modern conveyor systems. The viscoelastic layer is presumed to be one
dimensional in the sense of that of a Winkler foundation.
Explicit formulae for the resistance coefficient were developed and sample calculations
with material properties typical of a common backing material were made. The particular
material considered in the example calculations shows the typical peaking of the
indentation resistance at some point in the temperature/speed range. As an aid to design
and minimization of the power required for conveyor systems, the developed
methodology is directly usable for the evaluation of the performance of the backing
material, once the material properties are established through standard testing methods.
Rudolphi/Reicks
2/22/2006
References
1
M. Hager and A. Hintz, The energy-saving design of belts for long conveyor systems,
Bulk Solids Handling, 13, 4 (1993), pp. 749-758.
2
W.D. May, E.L. Morris and D. Atack, Rolling friction of a hard cylinder over a
viscoelastic material, Journal of Applied Physics, 30, 11 (1959), pp. 1713-1724.
3
C.O. Jonkers, The indentation rolling resistance of belt conveyors: A theoretical
approach, F&ouml;rdern und Heben, 30, 4 (1980), pp. 312-317.
4
C. Spaans, The calculation of the main resistance of belt conveyors, Bulk Solids
Handling, 11, 4 (1991), pp. 1-16.
5
G. Lodewijks, The rolling resistance of conveyor belts, Bulk Solids Handling, 15, 1
(1995) 15-22.
6
G. Lodewijks, Design of high speed belt conveyors, Bulk Solids Handling, 19, 4 (1999),
pp. 463-470.
7
K.L. Johnson, Contact Mechanics, Cambridge University Press, Cambridge, UK, 1985.
8
S.C. Hunter, The rolling contact of a rigid cylinder with a viscoelastic half space,
Journal of Applied Mechanics, 28 (1961), pp. 611-617.
9
L.W. Morland, A plane problem of rolling contact in linear viscoelasticity theory,
Journal of Applied Mechanics, 29 (1962), pp. 345-352.
10
A.S. Weinman and K.R. Rajagopal, Mechanical Response of Polymers: An
Introduction, Cambridge University Press, Cambridge, UK, 2000.
11
J.D. Ferry, Viscoelastic Properties of Polymers, 3rd Edition, Wiley, New York, 1980.
12
M. Williams, R. Landel and J. Ferry, The temperature dependence of relaxation
mechanisms in amorphous polymers and other glass-forming liquids, Journal of the
American Chemical Society, 77 (1955), p. 3701.
13
N. W. Tschoegl, The Phenomenological Theory of Linear Viscoelastic Behavior: An
Introduction, Springer, Berlin, 1989.
14
I. Emri and N.W. Tschoegl, Generating line spectra from experimental responses. Part
I: Relaxation modulus and creep compliance, Rheologica Acta, 32 (1993), pp. 311321.
Rudolphi/Reicks
2/22/2006
```